The history of textiles and ﬁbres spans thousands of years, beginning with the
style change from animal skins to the ﬁrst fabric used to clothe humanity. But
during the relatively short period of the past 50 years, the ﬁbre and textile
industries have undergone the most revolutionary changes and seen the most
remarkable innovations in their history. Chapter One discusses the most
important innovations together with the advent of the information industry.
In fact, it is the merger of these industries that has led to this book.
We are not talking merely of fabrics and textiles imparting information;
indeed, that has been occurring for many, many generations and numerous
examples exist from fabrics and tapestries that have told intricate tales of
warfare and family life and history, to those imparting information about the
wealth and social status of the owners of the fabrics. We are talking about
much more. Nor are we referring to fabrics that may have multifunctional
purposes, such as fashion and environmental protection, or rainwear, or those
fabrics providing resistance to a plethora of threats, such as ballistic, chemical
and ﬂame protection. These systems are all passive systems. No, we are
talking here about materials or structures that sense and react to environmental
stimuli, such as those from mechanical, thermal, chemical, magnetic or others.
We are talking ‘smart’ and ‘active’ systems. We are talking about the true
merger of the textile and information industries.
‘Smart textiles’ are made possible due to advances in many technologies
coupled with the advances in textile materials and structures. A partial list
includes biotechnology, information technology, microelectronics, wearable
computers, nanotechnology and microelectromechanical machines.
Many of the innovations in textile applications in the past 50 years have
started with military applications — from ﬁbreglass structures for radomes, to
fragment and bullet resistant body armour, to chemical agent protective
clothing, to ﬁbre-reinforced composites — indeed, many of our current defence
systems and advanced aircraft would not be possible without these materials.
So perhaps it is not surprising that the initial applications for smart textiles
have also come either directly from military R&D or from spin-oﬀs. Some of
the capabilities for smart textile systems for military applications are: sensing
and responding, for example to a biological or chemical sensor; power and
data transmission from wearable computers and polymeric batteries; trans-
mitting and receiving RF signals; automatic voice warning systems as to
‘dangers ahead’; ‘on-call’ latent reactants such as biocides or catalytic decon-
tamination in-situ for chemical and biological agents; and self-repairing materials.
In many cases the purpose of these systems is to provide both military and
civilian personnel engaged in high-risk applications with the most eﬀective
survivability technologies. They will thus be able to have superiority in
ﬁghtability, mobility, cognitive performance, and protection through materials
for combat clothing and equipment, which perform with intelligent reaction
to threats and situational needs. Thus, we will be providing high-risk personnel
with as many executable functions as possible, which require the fewest
possible actions on his/her part to initiate a response to a situational need.
This can be accomplished by converting traditional passive clothing and
equipment materials and systems into active systems that increase situational
awareness, communications, information technology, and generally improve
Some examples of these systems are body conformal antennas for integrated
radio equipment into clothing; power and data transmission — a personal area
network; ﬂexible photovoltaics integrated into textile fabrics; physiological
status monitoring to monitor hydration and nutritional status as well as the
more conventional heart monitoring; smart footwear to let you know where
you are and to convert and conserve energy; and, of course, phase change
materials for heating and cooling of the individual. Another application is the
weaving of sensors into parachutes to avoid obstacles and steer the parachutist
or the cargo load to precise locations.
There are, naturally, many more applications for ‘smart’ textiles than those
applied to military personnel, or civilian police, ﬁremen, and emergency
responders. Mountain climbers, sports personnel, businessmen with built-in
wearable microcomputers, and medical personnel will all beneﬁt from this
revolution in textiles.
You will learn of many more applications for ‘smart’ textiles in this book.
You will ﬁnd that the applications are limited only by your imagination and
the practical applications perhaps limited only by their cost. But we know
those costs will come down. So let your imagination soar. The current
worldwide textile industry is over 50 million metric tons per year, and if we are
able to capture only a measly 1% of that market, it is still worth more than
Dr Robert W. Lewis
Pushpa Bajaj, Toshihiro Hirai,
Department of Textile Technology, Department of Materials Chemistry,
Indian Institute of Technology, Faculty of Textile Science and
Hauz Khas, Technology,
New Delhi, Shinshu University,
India Tokida 3-15-1,
email@example.com Ueda-shi 386-8567,
Bischoﬀ Textile AG,
Switzerland Hartwig Hoecker,
bernhard.bischoﬀ@bischoﬀ-textil.com German Wool Research Institute at
Aachen University of Technology,
Philip J Brown, DWI,
School of Materials, Science & Veltmanplatz 8,
Engineering, D-52062 Aachen,
Clemson University, Germany
161 Sirrine Hall, firstname.lastname@example.org
Georgia Institute of Technology,
Elisabeth Heine, School of Textile and Fiber
Veltmanplatz 8, Atlanta,
D-52062 Aachen, GA 30332-0295,
So Yeon Kim, Seeram Ramakrishna,
School of Chemical Engineering, Faculty of Engineering,
College of Engineering, Department of Mechanical
Hanyang University, Engineering,
Haengdang-dong, Songdong-gu, National University of Singapore,
Seoul 133-791, 10 Kent Ridge Crescent,
Korea Singapore 119260
Young Moo Lee, Roland Seidl,
School of Chemical Engineering, Jakob Mueller Institute of Narrow
College of Engineering, Fabrics,
Hanyang University, Frick,
Haengdang-dong, Songdong-gu, Switzerland
Seoul 133-791, email@example.com
firstname.lastname@example.org Barbel Selm,
Swiss Federal Institute of Materials
Jin Kie Shim,
Heikki Mattila, School of Chemical Engineering,
Fibre Materials Science, College of Engineering,
Tampere University of Technology, Hanyang University,
PO Box 589, Haengdang-dong, Songdong-gu,
33101 Tampere, Seoul 133-791,
Sungmee Park, Hirofusa Shirai,
Georgia Institute of Technology, Faculty of Textile Science and
School of Textile and Fiber Technology,
Engineering, Shinshu University,
Atlanta, Tokida 3-15-1,
GA 30332-0295, Ueda-shi 386-8567,
Xiaoming Tao, Dongxiao Yang,
Institute of Textiles and Clothing, Department of Information and
The Hong Kong Polytechnic Electronic Engineering,
University, Zhejiang University,
Yuk Choi Road, Hangzhou 310027
Hung Hom, China
Hong Kong email@example.com
Devron P. Thibodeaux, Institute of Textiles and Clothing,
USDA, REE, ARS, MSA, The Hong Kong Polytechnic
1100 Robert E. Lee Boulevard, Yuk Choi Road,
New Orleans, Hung Hom,
LS 70124, Hong Kong
Institute of Functional Fibres,
Institute of Textiles and Clothing,
Tianjin Institute of Textile Science
The Hong Kong Polytechnic
Yuk Choi Road,
Tyrone L. Vigo, Faculty of Textile Science and
USDA, REE, ARS, MSA, Technology,
SRRC-CTCR, Shinshu University,
1100 Robert E. Lee Boulevard, Tokida 3-15-1,
New Orleans, Ueda-shi 386-8567,
LS 70124, Japan
Faculty of Textile Science and
The Editor wishes to thank the Hong Kong Polytechnic University for partial
support under the Area of Strategic Development Fund and Dr Dongxiao
Yang for assistance in compiling this book. The Editor also thanks all
contributing authors for their eﬀorts in making this book a reality.
List of contributors xiii
1 Smart technology for textiles and clothing
– introduction and overview 1
1.1 Introduction 1
1.2 Development of smart technology for textiles and clothing 3
1.3 Outline of the book 5
2 Electrically active polymer materials – application of
non-ionic polymer gel and elastomers for artiﬁcial
2.1 Introduction 7
2.2 Polymer materials as actuators or artiﬁcial muscle 9
2.3 Peculiarity of polymer gel actuator 10
2.4 Triggers for actuating polymer gels 10
2.5 Electro-active polymer gels as artiﬁcial muscles 15
2.6 From electro-active polymer gel to electro-active
elastomer with large deformation 28
2.7 Conclusions 30
3 Heat-storage and thermo-regulated textiles and
3.1 Development introduction 34
3.2 Basics of heat-storage materials 35
3.3 Manufacture of heat-storage and thermo-regulated textiles
and clothing 41
3.4 Properties of heat-storage and thermo-regulated textiles
and clothing 47
3.5 Application 52
3.6 Development trends 54
4 Thermally sensitive materials 58
4.1 Introduction 58
4.2 Thermal storage and thermal insulating ﬁbres 60
4.3 Thermal insulation through polymeric coatings 68
4.4 Designing of fabric assemblies 75
5 Cross-linked polyol ﬁbrous substrates as
multifunctional and multi-use intelligent materials 83
5.1 Introduction 83
5.2 Fibrous intelligent materials 83
5.3 Experimental 85
5.4 Results and discussion 86
5.5 Conclusions 91
6 Stimuli-responsive interpenetrating polymer network
hydrogels composed of poly(vinyl alcohol) and
poly(acrylic acid) 93
6.1 Introduction 93
6.2 Experimental 95
6.3 Results and discussion 97
6.4 Conclusions 106
7 Permeation control through stimuli-responsive
polymer membrane prepared by plasma and radiation
grafting techniques 109
7.1 Introduction 109
7.2 Experimental 110
7.3 Results and discussion 112
7.4 Conclusions 121
8 Mechanical properties of ﬁbre Bragg gratings 124
8.1 Introduction 124
8.2 Fabrication techniques 125
8.3 Mechanisms of FBG sensor fabrication 127
8.4 Mechanical properties 130
8.5 Inﬂuence of the UV irradiation on mechanical properties 133
8.6 Polymeric ﬁbre 141
8.7 Conclusions 145
9 Optical responses of FBG sensors under deformations 150
9.1 Introduction 150
9.2 Optical methodology for FBG sensors 151
9.3 Optical responses under tension 156
9.4 Optical responses under torsion 158
9.5 Optical responses under lateral compression 161
9.6 Optical responses under bending 165
9.7 Conclusions 166
10 Smart textile composites integrated with ﬁbre optic
10.1 Introduction 174
10.2 Optical ﬁbres and ﬁbre optic sensors 175
10.3 Principal analysis of embedded ﬁbre Bragg grating sensors 177
10.4 Simultaneous measurements of strain and temperature 181
10.5 Measurement eﬀectiveness 187
10.6 Reliability of FBGs 191
10.7 Error of strain measurement due to deviation of position and
10.8 Distributed measurement systems 195
10.9 Conclusions 195
11 Hollow ﬁbre membranes for gas separation 200
11.1 Historical overview of membranes for gas separation 200
11.2 Development of membranes for industrial gas separation 202
11.3 Theories of permeation processes 211
11.4 Phase inversion and hollow ﬁbre membrane formation 211
11.5 Future hollow ﬁbre membranes and industrial gas separation 214
12 Embroidery and smart textiles 218
12.1 Introduction 218
12.2 Basics of embroidery technology 218
12.3 Embroidery for technical applications — tailored ﬁbre
12.4 Embroidery technology used for medical textiles 221
12.5 Embroidered stamp — gag or innovation? 224
12.6 Summary 225
13 Adaptive and responsive textile structures (ARTS) 226
13.1 Introduction 226
13.2 Textiles in computing: the symbiotic relationship 226
13.3 The Georgia Tech Wearable Motherboard2+ 228
13.4 GTWM: contributions and potential applications 236
13.5 Emergence of a new paradigm: harnessing the opportunity 240
13.6 Conclusion 244
14 Wearable technology for snow clothing 246
14.1 Introduction 246
14.2 Key issues and performance requirements 247
14.3 The prototype 248
14.4 Conclusions 252
15 Bioprocessing for smart textiles and clothing 254
15.1 Introduction 254
15.2 Treatment of wool with enzymes 256
15.3 Treatment of cotton with enzymes 263
15.4 Enzymatic modiﬁcation of synthetic ﬁbres 270
15.5 Spider silk 270
15.6 ‘Intelligent’ ﬁbres 271
15.7 Conclusions 271
16 Tailor-made intelligent polymers for biomedical
16.1 Introduction 278
16.2 Fundamental aspects of shape memory materials 280
16.3 Concept of biodegradable shape memory polymers 281
16.4 Degradable thermoplastic elastomers having shape memory
16.5 Degradable polymer networks having shape memory
16.6 Conclusion and outlook 288
17 Textile scaffolds in tissue engineering 291
17.1 Introduction 291
17.2 Ideal scaﬀold system 295
17.3 Scaﬀold materials 296
17.4 Textile scaﬀolds 298
17.5 Conclusions 306
Smart technology for textiles and clothing –
introduction and overview
Since the nineteenth century, revolutionary changes have been occurring at an
unprecedented rate in many ﬁelds of science and technology, which have
profound impacts on every human being. Inventions of electronic chips,
computers, the Internet, the discovery and complete mapping of the human
genome, and many more, have transformed the entire world. The last century
also brought tremendous advances in the textile and clothing industry, which
has a history of many thousands of years. Solid foundations of scientiﬁc
understanding have been laid to guide the improved usage and processing
technology of natural ﬁbres and the manufacturing of synthetic ﬁbres. We
have learnt a lot from nature. Viscose rayon, nylon, polyester and other
synthetic ﬁbres were invented initially for the sake of mimicking their natural
counterparts. The technology has progressed so that synthetic ﬁbres and their
products surpass them in many aspects. Biological routes for synthesizing
polymers or textile processing represent an environmentally friendly, sustainable
way of utilizing natural resources. Design and processing with the aid of
computers, automation with remote centralized or distributed control, and
Internet-based integrated supply-chain management systems bring customers
closer to the very beginning of the chain than ever before.
Looking ahead, the future promises even more. What new capacities should
we expect as results of future developments? They should at least include
terascale, nanoscale, complexity, cognition and holism. The new capability of
terascale takes us three orders of magnitude beyond the present general-purpose
and generally accessible computing capabilities. In a very short time, we will be
connecting millions of systems and billions of information appliances to the
Internet. Technologies allowing over one trillion operations per second are on
the agenda for research. The technology in nanoscales will take us three orders
of magnitude below the size of most of today’s human-made devices. It will
allow us to arrange atoms and molecules inexpensively in most of the ways
2 Smart ﬁbres, fabrics and clothing
processing Electric and
1.1 A single cell living creature is an example of smart structures.
permitted by physical laws. It will let us make supercomputers that ﬁt on the
head of a ﬁbre, and ﬂeets of medical nanorobots smaller than a human cell to
eliminate cancers, infections, clogged arteries and even old age. Molecular
manufacturing will make exactly what it is supposed to make, and no
pollutants will be produced.
We are living in this exciting era and feeling the great impacts of technology
on the traditional textiles and clothing industry, which has such a long history.
Traditionally, many ﬁelds of science and engineering have been separate and
distinct. Recently, there has been considerable movement and convergence
between these ﬁelds of endeavour and the results have been astonishing. Smart
technology for materials and structures is one of these results.
What are smart materials and structures? Nature provides many examples
of smart structures. The simple single-celled living creature may highlight the
fundamentals. As shown in Fig. 1.1, various environmental conditions or
stimuli act on the outer layer. These conditions or stimuli may be in the form of
force, temperature, radiation, chemical reactions, electric and magnetic ﬁelds.
Sensors in the outer layer detect these eﬀects, and the resulting information is
conveyed for signal processing and interpretation, at which point the cell
reacts to these environmental conditions or stimuli in a number of ways, such
as movement, changing chemical composition and reproductive actions.
Nature has had billions of years and a vast laboratory to develop life, whereas
humankind has just begun to create smart materials and structures.
Smart materials and structures can be deﬁned as the materials and
structures that sense and react to environmental conditions or stimuli, such as
Smart technology for textiles and clothing – introduction and overview 3
those from mechanical, thermal, chemical, electrical, magnetic or other
sources. According to the manner of reaction, they can be divided into passive
smart, active smart and very smart materials. Passive smart materials can only
sense the environmental conditions or stimuli; active smart materials will
sense and react to the conditions or stimuli; very smart materials can sense,
react and adapt themselves accordingly. An even higher level of intelligence
can be achieved from those intelligent materials and structures capable of
responding or activated to perform a function in a manual or pre-programmed
Three components may be present in such materials: sensors, actuators and
controlling units. The sensors provide a nerve system to detect signals, thus in
a passive smart material, the existence of sensors is essential. The actuators act
upon the detected signal either directly or from a central control unit; together
with the sensors, they are the essential element for active smart materials. At
even higher levels, like very smart or intelligent materials, another kind of unit
is essential, which works like the brain, with cognition, reasoning and
activating capacities. Such textile materials and structures are becoming
possible as the result of a successful marriage of traditional textiles/clothing
technology with material science, structural mechanics, sensor and actuator
technology, advanced processing technology, communication, artiﬁcial in-
telligence, biology, etc.
1.2 Development of smart technology for textiles and
We have always been inspired to mimic nature in order to create our clothing
materials with higher levels of functions and smartness. The development of
microﬁbres is a very good example, starting from studying and mimicking silk
ﬁrst, then creating ﬁner and, in many ways, better ﬁbres. However, up to now,
most textiles and clothing have been lifeless. It would be wonderful to have
clothing like our skin, which is a layer of smart material. The skin has sensors
which can detect pressure, pain, temperature, etc. Together with our brain, it
can function intelligently with environmental stimuli. It generates large
quantities of sweat to cool our body when it is hot, and to stimulate blood
circulation when it gets cold. It changes its colour when exposed to a higher
level of sunlight, to protect our bodies. It is permeable, allowing moisture to
penetrate yet stopping unwanted species from getting in. The skin can shed,
repair and regenerate itself. To study then develop a smart material like our
skin is itself a very challenging task.
In the last decade, research and development in smart/intelligent materials
and structures have led to the birth of a wide range of novel smart products in
4 Smart ﬁbres, fabrics and clothing
aerospace, transportation, telecommunications, homes, buildings and infra-
structures. Although the technology as a whole is relatively new, some areas
have reached the stage where industrial application is both feasible and viable
for textiles and clothing.
Many exciting applications have been demonstrated worldwide. Extended
from the space programme, heat generating/storing ﬁbres/fabrics have now
been used in skiwear, shoes, sports helmets and insulation devices. Textile
fabrics and composites integrated with optical ﬁbre sensors have been used to
monitor the health of major bridges and buildings. The ﬁrst generation of
wearable motherboards has been developed, which has sensors integrated
inside garments and is capable of detecting injury and health information of
the wearer and transmitting such information remotely to a hospital. Shape
memory polymers have been applied to textiles in ﬁbre, ﬁlm and foam forms,
resulting in a range of high performance fabrics and garments, especially
sea-going garments. Fibre sensors, which are capable of measuring temperature,
strain/stress, gas, biological species and smell, are typical smart ﬁbres that can
be directly applied to textiles. Conductive polymer-based actuators have
achieved very high levels of energy density. Clothing with its own senses and
brain, like shoes and snow coats which are integrated with Global Positioning
System (GPS) and mobile phone technology, can tell the position of the wearer
and give him/her directions. Biological tissues and organs, like ears and noses,
can be grown from textile scaﬀolds made from biodegradable ﬁbres. Integrated
with nanomaterials, textiles can be imparted with very high energy absorption
capacity and other functions like stain prooﬁng, abrasion resistance, light
The challenges lie before us, as the research and development of smart
technology and its adoption by industries depend upon successful multidiscip-
linary teamwork, where the boundary of traditional disciplines becomes
blurred and cross-fertilization occurs at a rate much higher than that seen
previously. Some of the research areas can be grouped as follows:
∑ photo-sensitive materials
∑ conductive polymers
∑ thermal sensitive materials
∑ shape memory materials
∑ intelligent coating/membrane
∑ chemical responsive polymers
∑ mechanical responsive materials
∑ micro and nanomaterials.
Smart technology for textiles and clothing – introduction and overview 5
For signal transmission, processing and controls:
∑ neural network and control systems
∑ cognition theory and systems.
For integrated processes and products:
∑ wearable electronics and photonics
∑ adaptive and responsive structures
∑ tissue engineering
∑ chemical/drug releasing.
Research and development activities have been carried out worldwide, both
in academic/research institutions and companies. Research teams in North
American, European and Asian countries have been actively involved, with
noticeable outcomes either in the form of commercial products or research
1.3 Outline of the book
This edited book, being the ﬁrst on this topic, is intended to provide an
overview and review of the latest developments of smart technology for textiles
and clothing. Its targeted readers include academics, researchers, designers,
engineers in the area of textile and clothing product development, and senior
undergraduate and postgraduate students in colleges and universities. Also, it
may provide managers of textile and clothing companies with the latest
insights into technological developments in the ﬁeld.
The book has been contributed by a panel of international experts in the
ﬁeld, and covers many aspects of the cutting-edge research and development.
It comprises 17 chapters, which can be divided into four parts. The ﬁrst part
(Chapter 1) provides the background information on smart technology for
textiles and clothing and a brief overview of the developments and the book
structure. The second part involves material or ﬁbre-related topics from
Chapters 2 to 9. Chapter 2 is concerned with electrically active polymer
materials and the applications of non-ionic polymer gel and elastomers for
artiﬁcial muscles. Chapters 3 and 4 deal with thermal sensitive ﬁbres and
fabrics. Chapter 5 presents cross-linked polyol ﬁbrous substrates as multifunc-
tional and multi-use intelligent materials. Chapter 6 discusses stimuli-responsive
interpenetrating polymer network hydrogel. Chapter 7 is concerned with
permeation control through stimuli-responsive polymer membranes prepared
by plasma and radiation grafting techniques. Chapters 8 and 9 discuss the
6 Smart ﬁbres, fabrics and clothing
Table 1.1 Outline of the book
Chapter processing processes Bio-processes
no. Sensors/actuators and control and products and products
principles, manufacturing and properties of optical ﬁbre sensors, with
emphasis on ﬁbre Bragg grating sensors.
The third part contains ﬁve chapters, with a focus on integrating processes
and integrated structures. Chapter 10 provides an overview of the developments
and key issues in ﬁbre-optic smart textile composites. Chapter 11 presents
hollow ﬁbre membranes for gas separation. Chapter 12 describes embroidery
as one way of integrating ﬁbre-formed components into textile structures.
Chapters 13 and 14 are on wearable electronic and photonic technologies.
Chapter 13 provides insights on adaptive and responsive textile structures
(ARTS). Chapter 14 describes the development of an intelligent snowmobile suit.
The fourth part, embracing the last three chapters, is focused on
bioapplications. Chapter 15 outlines various bioprocesses for smart textiles
and clothing, and Chapter 16 concentrates on tailor-made intelligent polymers
for biomedical applications. Chapter 17 describes the applications of scaﬀolds
in tissue engineering, where various textile structures are used for cells to grow.
We have only seen a small portion of the emerging technology through the
window of this book. The possibilities oﬀered by this smart technology are
tremendous and widespread. Even as the book was being prepared, many new
advances were being achieved around the world. It is the hope of the editor and
contributors of this book that it will help researchers and designers of future
smart ﬁbres, textiles and clothing to make their dreams a reality.
Electrically active polymer materials –
application of non-ionic polymer gel and
elastomers for artiﬁcial muscles
TOSHIHIRO HIRAI, JIANMING ZHENG,
MASASHI WATANABE AND HIROFUSA SHIRAI
Many attempts have been made to functionalize polymer materials as
so-called ‘smart’ or ‘intelligent’ materials (see Fig. 2.1).— Artiﬁcial muscle or
intelligent actuators is one of the targets of such attempts. Historically,
actuator materials have been investigated mainly in inorganic compounds.
Particularly, triggers used for actuation are usually investigated in an electric
ﬁeld application because of the ease of control. Polymer materials investigated
from this point of view are very limited and have been known to generate much
smaller strain than inorganic materials.—
On the other hand, polymer materials such as polymer gels have been
known to generate huge strain by various triggers such as solvent exchange,
pH jump, temperature jump, etc., although the response and durability are
rather poor and they have not been used in practical actuators.
In the ﬁeld of mechanical engineering, the development of micromachining
procedure is facing the requirements of the technologies of microfabrication
and micro-device assembly, and there are high expectations of the emerging
smart materials that can greatly simplify the microfabrication process.—
Under these circumstances, the polymer gel actuator is mentioned as one of
the most likely candidates as a soft biological muscle-like material with large
deformation in spite of its poor durability. Much research has been done on
solid hard materials as actuators like poly(vinylidene ﬂuoride) (PVDF), which
is a well-known piezoelectrical polymer, and in which crystal structures play
critical role for the actuation and the induced strain is very small compared to
the gel artiﬁcial muscles that will be described in this chapter. Although PVDF
needs electrically oriented crystal structure in it, the materials that will be
discussed in this chapter do not require such a limitation.
Conventional electrically induced actuation has been carried out mostly on
ionic polymer gels. The reason is simply because ionic species are highly
8 Smart ﬁbres, fabrics and clothing
Trigger or stimuli Trigger or stimuli
Response or Response or
action (adaptation) action (adaptation)
2.1 Concepts of autonomic systems and materials. Three processes
(sensing, processing and actuation) are incorporated in materials (in one
system): (a) in autonomic materials, while they are separated and must be
uniﬁed by a controlling system; (b) in conventional autonomic systems.
responsive to the electric ﬁeld. Ionic gels have proved to be excellent
electroactive actuator materials.
However, we tried electrical actuation of non-ionic polymer gel or
elastomers. Why must non-ionic polymer gel be used for electrical actuation?
Because non-ionic polymer gel is superior to ionic polymer gel in several ways,
if it can be actuated by an electric ﬁeld. In ionic gel materials, electrolysis is
usually inevitable on the electrodes, and this is accompanied by a large electric
current and heat generation. In other words, elecrochemical consumption is
inevitable, although this fact has not been mentioned in most papers. In
non-ionic polymer gels, no such process is encountered, and this leads to the
good durability of the materials. In addition to these advantages, the
responding speed and magnitude of the deformation were found to be much
Electrically active polymer materials 9
faster (10 ms order) and larger (over 100%) than those induced in polyelectrolyte
gels. The motion reminds us of real biological muscle.
The concept of the mechanism is simple and can be applied to conventional
polymer materials, including materials commonly used in the ﬁbre and textile
industries. The concept is also applicable to non-ionic elastomers that do not
contain any solvent. The method we present will provide a promising way for
developing future artiﬁcial muscle. Several concepts developed by other
researchers and successfully used for actuating gels are also introduced in
comparison with our method.
2.2 Polymer materials as actuators or artiﬁcial muscle
Polymer gel is an electroactive polymer material. There are various types of
electroactive polymeric materials. As mentioned in the above section,
polyelectrolyte is one of them and is most commonly investigated as an
electroactive gel. We will come back to discuss this material in more detail in
the next section.
Ferroelectric polymer materials like PVDF or its derivatives are mentioned,
since they behave as ferroelectric materials (see Fig. 2.2). They have
crystallinity and the crystals show polymorphism by controlling the preparation
method. Much detailed work has been carried out on piezoelectric and/or
pyroelectric properties, together with their characteristics as electroactive
actuators. These materials have long been mentioned as typical electroactive
polymers. Through these materials, it is considered that the strain induced in
the polymer materials is not large. The electrostrictive coeﬃcient is known to
be small for polymers. These are non-ionic polymers and the induced strain
originates from the reorientation or the deformation of polarized crystallites in
the solid materials.
There is another type of electrically active polymer that is known as the
electroconductive polymer, in which polymer chains contain long conjugated
double bonds, and this chemical structure adds electroconductive properties
to the polymers. In these cases, the electrically induced deformation is
considered to have originated from the electrochemical reactions such as the
oxidation and reduction of the polymer chain. For the deformation, some
additives such as dopants have been known to be necessary for eﬀective
actuation. Therefore, the electrical actuation of these materials has been
2.2 Chemical structure of poly(vinylidene ﬂuoride) (PDVF).
10 Smart ﬁbres, fabrics and clothing
2.3 Chemical structures of (a) polypyrrole and (b) polyaniline.
investigated in the presence of water, similar to the case of polyelectrolyte gels.
Polypyrrole and polyaniline are typical examples (see Fig. 2.3).—
2.3 Peculiarity of polymer gel actuator
Polymer gels diﬀer in various ways from hard solid polymer materials. The
polymer chains in the gel are usually considered to be chemically or physically
cross-linked and to form a three-dimensional network structure. For instance,
polymer gel is usually a matter swollen with its good solvent, and the
characteristics are diversiﬁed from a nearly solid polymer almost to a solution
with very low polymer content but still maintaining its shape by itself. This
extreme diversity in physical properties widens the function of the gel (see Fig. 2.4).
From the standpoint of the actuator, the gel behaves like a conventional
solid actuator or biological muscle, or like a shapeless amoeba. The gels also
have various actuating modes, symmetric volume change with swelling and
de-swelling, asymmetric swelling behaviour, symmetric deformation and
asymmetric deformation (see Fig. 2.5). The strain induced in the gel can also be
extremely large, depending on the cross-link structure in the gel.
2.4 Triggers for actuating polymer gels
As can be expected from the diversiﬁed physical characteristics of the gel and
the wide variety of the actuating modes, there are various triggers for the
actuating polymer gels.
The triggers can be classiﬁed into two categories, chemical triggers and
physical triggers (see Fig. 2.6). As chemical triggers, solvent exchange includes
jumps in solvent polarity (e.g. from good solvent into poor solvent), in pH
(e.g. in weak polyelectrolyte gel from a dissociated condition into an associated
condition) and in ionic strength (utilizing salting-out or coagulation). These
Electrically active polymer materials 11
2.4 Extreme diversity in physical property widens the function of the gel.
2.5 Various actuating modes of polymer gels: (a) swelling and de-swelling,
(b) asymmetric swelling or de-swelling.
(a) Chemical triggers
oxidation and reduction
ionic strength change
(b) Physical triggers
magnetic field application
electric field application
2.6 Triggers for polymer and/or gel actuation can be classiﬁed into two
categories: chemical and physical.
12 Smart ﬁbres, fabrics and clothing
2.7 Chemical triggers including solvent exchange. These types
accompany swelling and de-swelling of the solvent, and the deformation
is usually symmetric as long as the gel has a homogeneous structure.
2.8 Temperature jump as a physical trigger: (a) poly(vinyl methyl ether)
and (b) poly(N-isopropyl acrylonide).
two types accompany swelling and de-swelling of the solvent, and the
deformation is usually symmetric as far as the gel has a homogeneous
structure (see Fig. 2.7). Temperature jump, which is a physical trigger, can also
induce symmetric deformation in particular polymer gels where the solubility
has a critical transition temperature. Typical examples are the gels of
poly(vinyl methyl ether) and poly(N-isopropyl acrylamide). These gels
have high water absorption at low temperatures and de-swell at the
characteristic critical temperature around 30—40 °C (see Fig. 2.8). The
transition temperature can be controlled by changing chemical structure.
In the case of urease immobilized gel, the addition of urea, a substrate of
Electrically active polymer materials 13
2.9 Chemical trigger can induce swelling and de-swelling of gel, e.g.
substrate of urease, urea, is changed into ammonia and the ammonia
induces swelling and de-swelling by varying pH.
2.10 Light-induced deformation of polymer ﬁlm. Example shown is the
case of PVC ﬁlm containing spyrobenzopyrane.
urease, induces swelling and deswelling by utilizing the pH change induced by
the enzyme reaction (see Fig. 2.9).
A physical trigger such as light irradiation is useful for actuating a gel in
which the light-induced reversible isomerization occurs and the isomerization
accompanies physical strain. In this case, the change is usually asymmetric
and the gel bends toward or against the direction of the irradiation, depending
on the photoinduced reaction (see Fig. 2.10).
In the case of electric ﬁeld application, the gels usually bend, because the
ﬁeld application induces asymmetric charge distribution and hence the
asymmetric strain in the gel. Asymmetric charge distribution can easily be
induced in polyelectrolyte gels, and this is why polyelectrolyte gel has mainly
been investigated as on electroactive polymer material (see Fig. 2.11).
Magnetic ﬁeld application can also induce a strain in a gel when a structure
or species sensitive to the magnetic ﬁeld is contained in it. We ﬁrst proposed
the idea of applying a super paramagnetic ﬂuid to a gel.— The gel was found
14 Smart ﬁbres, fabrics and clothing
2.11 Electrically induced deformation. In the case of electric ﬁeld
application, the gels usually bend, since ﬁeld application induces
asymmetric charge distribution and hence the asymmetric strain in the gel.
2.12 Magnetic ﬁeld active gel utilizing super paramagnetic property of a
ferro-ﬂuid-immobilized gel. , ferroﬂuid 75 wt %; *, ferroﬂuid 50 wt %;
ferroﬂuid 25 wt %.
Electrically active polymer materials 15
2.13 Magnetic ﬁeld induced large deformation. By turning the magnetic
ﬁeld (H) on and off, the gel deforms instantly.
to be sensitive to the magnetic ﬁeld gradient and to induce strain very
sensitively, and the structure change in the gel was investigated (see Fig. 2.12).
Zryhni and his coworkers investigated the same materials and found
discontinuous deformation of the gel by controlling the magnetic ﬁeld (see Fig.
2.5 Electro-active polymer gels as artiﬁcial muscles
Amongst the polymeric actuator materials mentioned above, polymer gel has
an important property as a huge strain generating material. As mentioned in
the previous section, the electric ﬁeld is one of the most attractive triggers for
practical actuation. Electroactivity has been mentioned in connection with
polyelectrolyte gels, since they contain ionic species. However, ionic species
are not only sensitive to an electric ﬁeld, but also usually electrochemically
active, and accompany electrolysis on the electrodes. Electrochemical reactions
often result in increased current and heat generation. These processes only
dissipate energy, and do not contribute to strain generation. Thus, elec-
trochemical reactions are an undesirable process in most cases. In spite of their
many diﬃculties for practical actuators, polyelectrolyte gels and related
materials still remain at the forefront of electroactive polymer materials.
To overcome diﬃculties in polyelectrolytes, such as electrochemical
consumption on the electrodes, we investigated the electroactive properties of
the non-ionic polymer gel.
2.5.1 Electroactive polyelectrolyte gels
As pointed out in the previous section, polyelectrolyte gels have been
investigated as electroactive actuator materials. The concept originates from
the presence of electroactive ionic species in the gels. The ionic species can
16 Smart ﬁbres, fabrics and clothing
2.14 Bending deformation of a poly(acrylonide-co-sodium acrylate) gel in
aqueous solution. Bending direction is changed with sodium acrylate
content in the gel. Acrylic acid content was controlled by hydrolysing
poly(acrylonide) gel. The mechanism was explained with the results
shown in Fig. 2.15.
2.15 Electrically induced asymmetric deformation of a
poly(acrylonide-co-sodium acrylate) gel. Sodium acrylate content is
(a) low, and (b) high. In (a) the gel shrinks on anode side, but swells in (b).
migrate and form localized distribution and/or electrochemical reactions in
the gel, which cause its deformation.
22.214.171.124 Poly(acrylic acid) gel
Among polyelectrolyte gels, poly(acrylic acid) (PAA) gel was the ﬁrst polyelec-
trolyte investigated as an electroactive polymer gel. Shiga et al. found that
PAA gel can be deformed by DC electric ﬁeld application in the presence of
salt.— A PAA gel rod was immersed in the saline aqueous solution (see Fig.
2.14). The platinum electrodes were apart from the gel surface, and the DC
ﬁeld was applied from both sides of the gel. Shiga et al. found a slow bending
motion of the gel, the magnitude of bending depending on the salt and its
concentration. They also found an asymmetric deformation of the gel, when
the ﬁeld was applied apart from both ends of the gel rod (see Fig. 2.15). In this
case, the gel shrinks at one end and swells at the other end. The motion is
explained by asymmetric swelling behaviour under the ﬁeld. The deformation
is explained by the following equation derived by Flory:
: ; ; [2.1]
Electrically active polymer materials 17
2.16 Gel ﬁnger in aqueous solution. Polymer gel contains poly(acrylic)
acid and poly(vinyl alchohol). One electrode is occluded in the gel, and the
other electrode is exposed in the solution.
: 9 [ln(1 9 ) ; ; x ]RT/V [2.2]
: ( 9 /2)RT /V [2.3]
: ( c 9 c )RT [2.4]
where is the overall osmotic pressure which is the summation of the three
types of osmotic pressure, , and , which originate from the interaction
between the polymer chain and solvent, from the rubber elasticity of the gel,
and from the concentration diﬀerences of the ionic species inside and outside
the gel, respectively. The parameters , x, V , , V , c , c , R and T are the
C G H
polymer volume fraction, the interaction parameter between polymer and
solvent, the volume of dried polymer, the eﬀective chain number in the
network, the molar volume of the solvent, the concentration of species i in the
gel, the concentration of species j in outer solution, the gas constant and the
absolute temperature, respectively.
The process was considered to originate from an osmotic pressure gap
induced by the localization of ionic species of diﬀerent solvation power. In this
movement, electrolysis usually occurred on the electrodes. Shiga et al. optimized
the preparation method in order to overcome the diﬃculty. They put the
electrodes on the gel surface, and successfully demonstrated the gel ﬁnger in
aqueous solution (see Fig. 2.16).
18 Smart ﬁbres, fabrics and clothing
2.17 Association and dissociation of polyelectrolyte gel of
poly(2-acrylamido-2-methylpropanesulfonic acid) (PAMPS) with cationic
surfactant was found to undergo worm-like motility in aqueous solution.
126.96.36.199 Poly(2-acrylamido-2-methylpropanesulfonic acid) gel
Poly(2-acrylamido-2-methylpropanesulfonic acid) (PAMPS) gel was found to
undergo worm-like motility (see Fig. 2.17).— The principle of this deformation
is based on an electrokinetic molecular assembly reaction of surfactant molecules
on the hydrogel, caused by both electrostatic and hydrophobic interactions
and resulting in anisotropic contraction to give bending towards the anode.
When the ﬁeld is reversed, the surfactant admolecules on the surface of the gel
lift oﬀ and travel away electrically towards the anode. Instead, new surfactant
molecules approach from the opposite side of the gel and form the complex
preferentially on that side of the gel, thus stretching the gel. Surfactants such
as N-dodecylpyridinium chloride (Cl PyCl) were used, which adsorbed within
a second and is easily calculated to give a complex formation ratio less than
1 ; 10, explaining that the quick and large bending under an electric ﬁeld is
dominated only by the surface complexation and shrinkage of the gel.
Electrically active polymer materials 19
2.18 Ion-exchange polymer–metal composite ﬁlm of Naﬁon, of Dupont or
Flemion of Asahi Glass Co. Ltd. can bend remarkably by applying low
188.8.131.52 Perﬂuorosulfonate ionomer gel
A hydrogel of perﬂuorosulfonate ionomer (Naﬁon of Dupont) ﬁlm, thickness
of ca. 0.2 mm, was found to be an eﬀective electroactive material (see Fig.
2.18).— This material can be actuated by a DC ﬁeld application of low
voltage such as 3 volts. Success was attained by the development of the
chemical deposition of the electrode on the membrane surface. The principle
of the deforming mechanism is somewhat similar to the case of other
polyelectrolyte gels. That is, the membrane requires the presence of water and
salts, and an encounter of electrochemical consumption is principally inevitable.
However, the response time and durability are much higher than with the
other gel materials. Moreover, the actuating process is not seriously aﬀected
by electrochemical reactions, provided the operating conditions are adequately
controlled. Improvement of the eﬃciency can be considered to originate from
the chemical structure of the membrane, and the coexistence of the strong
hydrophobicity and strong hydrophilicity in a polymer chain.
2.5.2 Electroactive non-ionic polymer gels
Reviewing the above-mentioned materials, one of the serious defects of
polyelectrolyte gels is the electrochemical consumption on the electrode under
an electric ﬁeld application. The electrochemical consumption causes poor
durability of the polyelectrolyte gels and limits their application ﬁelds.
Therefore, the authors tried to utilize non-ionic polymer gels as actuating
materials with large deformation. The results show that the idea works in a far
20 Smart ﬁbres, fabrics and clothing
2.19 Dependence of strain in the direction of the ﬁeld on the electric ﬁeld.
more eﬃcient manner than expected, but the mechanism turned out to be not
the same as they expected initially. The feature will be described below in a
184.108.40.206 Strain in the direction of the ﬁeld
Poly(vinyl alcohol)—DMSO gel was prepared by combining physical cross-
linking and chemical cross-linking with glutaraldehyde (GA). After the chemical
cross-linking, the physical cross-links were eliminated by exchanging solvent
into pure DMSO. The chemically cross-linked gel thus obtained has an
electronically homogeneous structure. Therefore, the PVA—DMSO gel has no
intrinsic polarization in its structure, and electrostrictive strain generation is
expected by applying a DC electric ﬁeld. The results agree with this expectation,
and the strain is proportional to the square of the ﬁeld (see Fig. 2.19). The
strain observed reached over 7% in the direction of the ﬁeld. The response
time is very fast, the large strain is attained within 0.1 s, and the shape of the
gel is instantly restored by turning oﬀ the ﬁeld. The current observed is
around 1 mA at 250 V/mm, which is much smaller than those of polyelectrolyte
gels. The current can be depressed by further puriﬁcation of the polymer and
solvent. This performance is much faster than conventional polyelectrolyte
gels. We can demonstrate the electro-activated quick strain in the ﬂapping
motion by amplifying the strain by 300 times. It is suggested that the ﬂapping
motion be accelerated up to 10 Hz, though the demonstration was carried out
at 2 Hz (see Fig. 2.20).
Electrically active polymer materials 21
Rod (12.5 cm)
with a span
DC power of 10 cm
Gel (thickness = 4 mm)
2.20 Flapping motion induced by an electrostrictive deformation of a
non-ionic polymer gel swollen with a dielectric solvent.
2.21 Structure of dimethylsulfoxide and its orientation by an electric ﬁeld.
Polarized Raman spectroscopy can be employed for investigating the
molecular orientation under the ﬁeld.
220.127.116.11 Electrical orientation of solvent
The strain induced in the direction of the ﬁeld cannot be explained by the
electrostatic attractive force between the electrodes. The eﬀect of the electrostatic
ﬁeld was expected to be less than 25% of the observed strain under our
experimental conditions. We therefore have to ﬁnd another explanation for
the strain generation in the gel.
Initially, we expected the orientation of solvent molecule under an electric
ﬁeld to lead the strain generation in the gel, through the changes of interactions
between solvent and solute polymer, which forms the gel network.
In order to observe the eﬀect of the electric ﬁeld on the orientation of the
solvent, DMSO, Raman spectroscopy was employed. The molecule has a
strong dipole moment, and can be expected to orient along the ﬁeld direction
(see Fig. 2.21). It is oriented very eﬃciently even in relatively low electric
ﬁelds, but the orientation decreases over the maximum ﬁeld intensity (see Fig.
2.22). The deformation of the gel becomes greater in the region of the higher
ﬁeld than that of the maximum orientation, suggesting that the solvent
orientation is not directly related to the deformation of the gel.
22 Smart ﬁbres, fabrics and clothing
Anisotropy of scattering intensity
0 25 50 75 100
2.22 Electrically induced orientation of DMSO. DMSO orients very
efﬁciently even in relatively low electric ﬁeld, but the orientation decreases
over the maximum ﬁeld intensity.
18.104.22.168 Bending and crawling motion accompanying huge strain
In observing the contraction along the direction of an electric ﬁeld, brass
plates were used as electrodes. The strain in the perpendicular direction of the
ﬁeld was also observable. In these measurements, the bending deformation of
the gels was prevented or completely depressed.
When we carefully observed the gel deformation, solvent ﬂow and some
asymmetric deformation was suggested in the gel. But conventional electrodes
or a thin metal sheet of 10 m thickness did not lead to any eﬀective deformation.
We used very thin gold electrodes whose thickness was 0.1 m, and covered
both surfaces of the gel with the thin metal sheet. The metal sheet is soft
enough and does not disturb even a slight deformation of the gel.
By applying a DC electric ﬁeld to the gel, the gel bent swiftly and held the
deformation as far as the ﬁeld was on (see Fig. 2.23).— The bending was
completed within 60 ms, and the bending angle reached over 90 degrees. By
turning oﬀ the ﬁeld, the strain was released instantly, and the gel resumed its
original shape (see Fig. 2.24). The curvature turned out to be proportional to
the square of the ﬁeld (see Fig. 2.25).
Taking the gel size (length 1 cm, width 5 mm and thickness 2 mm) into
account, and assuming the gel volume does not change in the deformation, the
strain in the gel can be estimated to be over 140% in length. The electric
current observed in this motion was less than 30 A under the ﬁeld of 500 V/mm.
This response and the huge strain attained in the PVA—DMSO gel is the
Electrically active polymer materials 23
(thickness = 2 mm
width = 5 mm
length = 1 cm)
Thin gold electrodes
(thickness = 0.1 m)
2.23 Assembling an electroactive non-ionic gel. The metal sheet was soft
enough and does not disturb even a slight deformation of the gel.
2.24 Swift bending of a non-ionic polymer gel. By applying a DC electric
ﬁeld to the gel, the gel bent swiftly and sustained the deformation while
the ﬁeld was on.
largest value among the electroactive polymer gel materials reported so far.
The low current suggests that there is much less energy loss in this motion
compared with the conventional polyelectrolyte gels. The energy loss as heat
was much less than that of Naﬁon or Flemion membrane overall, therefore it
is far less when the size (thickness and surface area) of the gel is taken into
24 Smart ﬁbres, fabrics and clothing
R (mm 1)
50 100 200 300
2.25 Dependence of bending curvature on an electric ﬁeld.
2.26 Crawling motion of a non-ionic polymer gel.
The gel could also show a crawling-type deformation. This is a novel type
of motion. The crawling motion was observed when a naked gel was placed on
an electrode stripe array. The motion was completed in ca. 1 second (see Fig. 2.26).
22.214.171.124 Origin of the asymmetric pressure distribution in the gel
Such a remarkable swift bending or crawling of a non-ionic polymer gel
cannot be explained by osmotic pressure gradient, which is usually considered
to be the reason for electrically induced bending in polyelectrolyte gel. As
pointed out in the previous section, the solvent ﬂow was suggested in the gel.
We investigated the eﬀect of an electric ﬁeld on its ﬂowing property.
Electrically active polymer materials 25
2.27 Electric ﬁeld-induced ﬂow of a dielectric solvent. A pair of cone-like
electrodes were dipped in a circular tray ﬁlled with DMSO.
Flow rate (mm/s)
0 200 400
2.28 Dependence of a ﬂow rate on an electric ﬁeld. The ﬂow rate was
proportionally increased with the square of the ﬁeld.
A pair of comb-like electrodes were dipped in a circular tray ﬁlled with
DMSO (see Fig. 2.27). When a DC ﬁeld was applied, the solvent started
ﬂowing from anode to cathode. The ﬂowing rate was measured by using
polystyrene powder ﬂoating on the solvent as a probe. The ﬂow rate increased
proportionally with the square of the ﬁeld (Fig. 2.28). This result suggests that
the pressure gradient is generated between the electrodes.
In order to establish a quantitative estimation of the pressure gradient, a
theoretical treatment was carried out under some hypotheses shown below:
1 Only one value of ion mobility exhibits for a kind of ion.
2 The turbulence in the gel can be neglected for the calculations of the
3 The ionizing and accelerating electrodes do not interfere with pressure
26 Smart ﬁbres, fabrics and clothing
2.29 Solvent DMSO is drawn up between the electrodes.
4 Although only a very small resultant current exists, it is enough to determine
the ﬁeld distribution.
5 Diﬀerent types of ions do not interfere with each other in the pressure
6 Surface charges on solvent boundaries have a negligible eﬀect on ion
current and ﬁeld distribution.
The following equation was deduced for the pressure distribution in a gel:
9 V9V x
p(x) 9 p(0) : [2.5]
8 d d
where p(x) 9 p(0), , V, V and d are pressure gaps between the two positions 0
(on the gel surface) and x (at x in the gel from the gel surface) in the direction of
the ﬁeld, dielectric constant, voltages on the gel surface and at x in the gel, and
the thickness of the gel, respectively.
This equation suggests that the pressure gradient generated in the gel is
proportional to the dielectric constant of the gel and to the square of an
electric ﬁeld. As the solvent content of the gel is ca. 98% in our experimental
system, the dielectric constant of the gel can be assumed to be the same as that
of the solvent. By taking the bending elasticity of the gel and the estimated
pressure, we could attain excellent agreement between our experimental data
and theoretical estimation (see Fig. 2.29).
In order to see the eﬀect of the polymer on the electrically induced deformation,
another type of experiment was carried out. A pair of plate electrodes were
Electrically active polymer materials 27
Height pulled up (mm)
0 200 400 600 800 1000
E (V/1.5 mm)
2.30 Dependence of drawn-up height of DMSO on the electric ﬁeld.
dipped in the solvent, and the DC ﬁeld was applied between the electrodes.
The solvent was pulled up between the electrodes (Fig. 2.30). The height was
theoretically estimated by the following equation:
h : ( 9 )(V/d)/ g [2.6]
where h, , , V, d, and g are liquid surface height, dielectric constant of the
gel, dielectric constant of vacuum, voltage applied, distance between the
electrodes, density of the gel and gravitational constant.
The curve in Fig. 2.30 was calculated to be one, and is in good agreement
with the experimental data. However, when we used a DMSO solution of
PVA, the height was much less than that observed in the solvent and,
furthermore, was extremely asymmetric on both electrodes (see Fig. 2.31). The
solution tends to climb up onto the cathode surface, but not onto the anode,
suggesting that the above equation is no longer applicable for the polymer
These phenomena imply that the polymer solution has the tendency to
retard the discharging process. The discharge retardation causes the accumu-
lation of the charge on the cathode side in the gel and enhances the pressure
gap between the cathode side and the anode side in the gel. Thus, the presence
of the polymer network also plays an important role in eﬃcient bending
For more detailed analysis, further quantitative investigation must be
28 Smart ﬁbres, fabrics and clothing
2.31 Climbing of PVA–DMSO solution onto an electrode under the ﬁeld.
126.96.36.199 Applicability of the ‘charge-injected solvent drag’ method for conventional
The concept proposed in the previous section can be described as the
‘charge-injected solvent drag’ method. The advantage of the method is its
wide applicability to conventional non-ionic polymeric gel-like materials. We
have been working on several non-ionic materials for soft artiﬁcial muscles
that can be actuated in air.
Here, the case of poly(vinyl chloride) (PVC) will be shown brieﬂy. In the
case of PVC, we used plasticizers as solvent. Although tetrahydrofurane is a
good solvent for PVC, its boiling point is too low for the preparation of the
stable gel at ambient temperature in air. In the example shown, the PVC gel
plasticized with dioctylphthalate (DOP) was found to creep reversibly like an
amoeba by turning on and oﬀ the electric ﬁeld (see Fig. 2.32). The electrically
induced deformation was suggested to be the asymmetric distribution of the
injected charge. The mechanism is somewhat similar, but not the same, to that
for the non-ionic polymer gel, since the solvent ﬂow has not been conﬁrmed in
2.6 From electro-active polymer gel to electro-active
elastomer with large deformation
Non-ionic polymer gel swollen with dielectric solvent is shown to be extremely
deformed, as is the non-ionic polymer plasticized with non-ionic plasticizer.
Electrically active polymer materials 29
2.32 Creeping motion of poly(vinyl chloride) plasticized with
dioctylphthalate. PVC gel plasticized with dioctylphthalate (DOP) was
found to creep reversibly like an amoeba by turning the electric ﬁeld on
The mechanism suggested for the gel actuation was ‘charge-injected solvent
drag’, and that for the plasticized polymer was ‘asymmetric charge distribution
of injected charge’.
The latter mechanism can be applied to the non-ionic elastomers in
which the motion of the polymer chain is relatively free and so is the migra-
tion of the injected charges. The migration of the injected charge and the bal-
ance of the charging and discharging rates must be a critical factor to the
deformation provided the electrostatic interaction is a major factor in the
The experimental results on polyurethane elastomers support the concept
described above.— In addition to our expectations, some novel features of
the motion are being clariﬁed in detail, such as memory eﬀect, bending
direction control, and so on (Fig. 2.33).
30 Smart ﬁbres, fabrics and clothing
Highly swollen gel Plasticized polymer
Swift bending motion Creeping motion Swift motion
Crawling motion Huge deformation Memory effect
Charge injected solvent drag Bending direction control
Poor durability Huge deformation
2.33 Wide span of large deforming non-ionic electro-active actuator
materials from polymer gel, through plasticized polymer, to elastomer
with no additives. A prosperous future for the conventional non-ionic
polymer materials as autonomic materials can be expected.
In this chapter, various types of electroactive polymers were introduced. Some
of them have a long history as electroactive materials. Recently, however,
polymer gels and/or elastomers, which have no intrinsic polarization in their
structure and do not contain any ionic species either, have been found to show
huge strain by applying electric ﬁelds with a low electric current. Energy
dissipation occurring as heat is much less than the conventional polyelectrolyte
materials. The concepts of ‘charge-injected solvent drag’ and ‘asymmetric
charge distribution of injected charge’ are proposed as a possible mechanism
of the huge deformation. These concepts can be applied to various non-ionic
conventional polymers. The author strongly expects that the concepts expand
the ﬁeld of actuator to that of practical artiﬁcial muscle, and contribute to the
development of the micro-machine or nano-machine in the future.
The work described in this article is partly supported by Grants-in-Aid for
COE Research (10CE2003) and Scientiﬁc Research B(12450382), and by the
Regional Science Promoter Program of Nagano Prefecture. The author (TH)
expresses his sincere thanks for the support.
1 Polymer Gels. Fundamentals and Biomedical Applications, ed. DeRossi, Danilo,
Kajiwara, Kanji, Osada, Yoshihito and Yamauchi, Aizo, Prenum (1991).
2 Osada, Y and Kajiwara K (eds), Gel Handbook, NTS Publishing Co. Ltd. (1997).
3 Handbook of New Actuators for Accurate Controlling, Supervised by K Uchino, Fuji
Electrically active polymer materials 31
Technosystem Publishing Co. Ltd. (1994).
4 Organic Polymer Gels, Kikan Kagaku Sosetsu, No. 8, ed. by the Chemical Society of
Japan, Gakkai Shuppan Center (1990).
5 Recent Trends and Development of Polymer Gels — For Professionals in the Advanced
Technology Field, Supervised by Y Osada and Lin Wang, CMC Co. Ltd. (1995).
6 Uchino K, Piezo/Electrostrictive Materials, Morikita Publishing Co. Ltd. (1986).
7 Jikken Kagaku Koza (Experimental Chemistry Series), ed. by the Chemical Society
of Japan, 9 (1991).
8 Miyata S and Furukawa T, Ferroelectric Polymers, ed. by Polymer Society of
Japan, New Polymer Materials, One Point Series 14, Kyoritsu Publishing Co. Ltd.
9 Micromachine Research Laboratory, The University of Tokyo, Super Technology —
Micromachine, NTT Publishing Co. (1993).
10 Fujita H, The World of Micromachine, K Books Series 85, Kogyochosakai
Publishing Co. Ltd. (1992).
11 Actuator Research Group, New Actuators Targeting Microworld, K Books Series
103, Kogyochosakai Publishing Co. Ltd. (1994).
12 Kinoshita G, Soft Machine, New Corona Series 16, Corona Publishing Co. Ltd. (1992).
13 Bar-Cohen Y, ‘Electroactive Polymer Actuators and Devices’, Proceedings of SPIE,
14 Bohannan G W, Schmidt V H, Conant R J, Hallenberg J H, Nelson C, Childs A,
Lukes C, Ballensky J, Wehri J, Tikalsky B and McKenzie E, ‘Piezoelectric polymer
actuators in a vibration isolation application’, Proceedings of SPIE, 3987, 331 (2000).
15 Wang H, Zhang Q M, Cross L E and Sykes A O, ‘Piezoelectric, dielectric, and
elastic properties of poly(vinylidene ﬂuoride/triﬂuoroethylene), J. Appl. Phys., 74,
16 Mazzoldi A and DeRossi D, ‘Conductive polymer based structures for a steerable
catheter’, Proceedings of SPIE, 3987, 271 (1999).
17 MacDiarmid A G and Epstein A J, ‘Polyanilines: A novel class of conducting
polymers’, Faraday Discussions, 1989, n. 88, 317.
18 Baughman R H, ‘Conducting polymer artiﬁcial muscles’, Synthetic Metals, 78, 339
19 Gandhi M R, Murray P, Spinks G M and Wallace G G, ‘Mechanism of
electromechanical actuation in polypyrrole’, Synthetic Metals, 73, 247 (1995).
20 Hirai T, Hanaoka K, Suzuki T and Hayashi S, ‘Preparation of oriented hydrogel
membrane’, Kobunshi Ronbunshu, 49, 613 (1989).
21 Hirai T, ‘Artiﬁcial muscle’, Shin-Sozai (New Materials), No. 4 (1992).
22 Suzuki M, ‘Nonlinear mechanochemical systems’, Nippon Gomu Kyokaishi, 60, 702
23 Osada Y, ‘Chemical valves and gel actuators’, Adv. Mater., 3, 107 (1991).
24 Hirai T, Asada Y, Suzuki T, Hayashi S and Nambu M, ‘Studies on elastic hydrogel
membrane. I. Eﬀect of preparation conditions on the membrane performance’, J.
Appl. Polym. Sci., 38, 491 (1989).
25 Hirasa O, Morishita Y, Onomura R, Ichijo H and Yamauchi I, ‘Preparation and
mechanical properties of thermo-responsive ﬁbrous hydrogels made from poly(vinyl
methyl ethers)’, Kobunshi Ronbunshu, 46, 661 (1989).
26 Okano T, Bae Y H and Kim S W, ‘Temperature dependence of swelling of
32 Smart ﬁbres, fabrics and clothing
crosslinked poly(N,N-alkyl substituted acrylamides in water’, J. Controlled
Release, 11, 255 (1990).
27 Tanaka T, Sato E, Hirokawa Y, Hirotsu S and Peeternians J, ‘Critical kinetics of
volume phase transition of gels’, Phys. Rev. Lett., 55, 2455 (1985).
28 Tokita M and Tanaka T, ‘Reversible decrease of gel-solvent friction’, Science, 253,
29 Kokufuta E, Zhang Y-Q and Tanaka T, ‘Saccharide-sensitive phase transition of a
lectin-loaded gel’, Nature, 351, 302 (1991).
30 Kokufuta E, ‘New development of immobilized enzymes’, Hyoumen (Surfaces), 29,
31 Tanaka T, ‘Phase transitions in ionic gels’, Phys. Rev. Lett., 45, 1636—1639 (1980).
32 Irie M, ‘Photoresponsive polymers’, Adv. Polymer Sci., 28 (1989).
33 Takamizawa T, Hirai T, Hayashi S and Hirai M, ‘Magnetostriction of a gel
immobilizing superparamagnetic ﬂuid’, Proceedings of International Symposium on
Fiber Science and Technology (ISF’94), in Yokohama, 293 (1994).
34 Hirai T, ‘Electrically and magnetically active gel’, ZairyoKagaku (Materials
Science), 32, 59 (1995).
35 Hirai T, Takamizawa T and Hayashi S, ‘Structural change induced in the gel
immobilizing superparamagnetic ﬂuid’, Polym. Preprints, Jpn., 43, 3126 (1993).
36 Zryhni M, Barsi L and Buki A, ‘Deformation of ferrogels induced by nonuniform
magnetic ﬁelds’, J. Chem. Phys., 104, 20 (1996).
37 Zryhni M, Barsi L, Szabo D and Kilian H-G, ‘Direct observation of abrupt shape
transition in ferrogels induced by nonuniform magnetic ﬁeld’, J. Chem. Phys., 106,
38 Zryhni M and Horkai F, ‘On the thermodynamics of chemomechanical energy
conversion realised by neutral gels’, J. Intell. Mater. Syst. and Struct., 4, 190 (1993).
39 Shiga T, Hirose Y, Okada A and Kurauchi T, ‘Bending of high-strength polymer gel
in an electric ﬁeld’, Kobunshi Ronbunshu, 46, 709 (1989).
40 Shiga T, Hirose Y, Okada A and Kurauchi T, ‘Bending of ionic polymer gel
caused by swelling under sinusoidally varying electric ﬁelds’, J. Appl. Polym. Sci., 47,
41 Shiga T, Fukumori K, Hirose Y, Okada A and Kurauchi T, ‘Plused NMR study of
the structure of poly(vinyl alcohol)—poly(sodium acrylate) composite hydrogel’, J.
Polym. Sci.: Part B: Polym. Phys., 32, 85 (1994).
42 Osada Y, Okuzaki H and Hori H, ‘A polymer gel with electrically driven motility’,
Nature, 355, 242 (1992).
43 Gong J P, Kawakami I, Sergeyev V G and Osada Y, ‘Electroconductive organogel.
3. Preparation and properties of a charge-transfer complex gel in an organic
solvent’, Macromolecules, 24, 5246 (1991).
44 Gong J P, Kawakami I and Osada Y, ‘Electroconductive organogel. 4. Electrodriven
chemomechanical behaviors of charge-transfer complex gel in organic solvent’,
Macromolecules, 24, 6582 (1991).
45 Oguro K, Kawami Y and Takanaka H, ‘An actuator element of polymer electrolyte
gel membrane-electrode composite’, Bull. Government Industrial Research Institute
Osaka, 43, 21 (1992).
46 Oguro K, Fujiwara N, Asaka K, Onishi K and Sewa S, ‘Polymer electrolyte
actuator with gold electrodes’, Proceedings of SPIE, 3669, 64 (1999).
Electrically active polymer materials 33
47 Mojarrad M and Shahinpoor M, ‘Noiseless propulsion for swimming robotic
structures using polyelectrolyte ion-exchange membrane’, Proc. SPIE, 1996 North
American Conference on Smart Structures and Materials, 2716, Paper no. 27, 183
48 Shahinpoor M, ‘Electro-mechanics of ion-elastic beams as electrically-controllable
artiﬁcial muscles’, Proc. SPIE, Electroactive polymer actuators and devices, 3669,
49 Hirai T, Maruyama H, Suzuki T and Hayashi S, ‘Shape memorizing properties of
poly(vinyl alcohol) hydrogel’, J. Appl. Polym. Sci., 45, 1849 (1992).
50 Hirai T, Nemoto H, Hirai M and Hayashi S, ‘Electrostriction of poly(vinyl alcohol)
gel — a possible application for artiﬁcial muscle’, J. Appl. Polym. Sci., 53, 79 (1994).
51 Errede L A, Osada Y and Tiers V D, ‘Molecular interpretation of chemo-mechanical
reponses in polymer liquid systems’, J. Intell. Mater. Systems Struct., 4, 2, 161 (1993).
52 Hirai M, Hirai T, Sukumoda A, Nemoto H, Amemiya Y, Kobayashi K and Ueki T,
‘Electrically induced reversible structural change of a highly swollen polymer gel
network’, J. Chem. Soc., Faraday Trans., 91, 473 (1995).
53 Hirai T and Hirai M, Polymer Sensors and Actuators, ed. Y Osada and D E DeRossi,
Chapter 8, p. 245, Springer-Verlag, Berlin, Heidelberg (2000).
54 Hirai T, Jianming Zheng and Watanabe M, Proc. of SPIE, SPIE’s 6th Annual
International Symposium on Smart Structures and Materials, Electro-active
Polymer Actuators and Devices, 3669, 209 (1999).
55 Zheng J, Watanabe M, Shirai H and Hirai T, ‘Electrically induced rapid
deformation of nonionic gel’, Chem. Lett., 500—501 (2000).
56 Hirai T, Zheng J, Watanabe M and Shirai H, ‘Autonomic gel and its application as
artiﬁcial muscle’, Zairyo Kagaku (Materials Science), 36, 186 (2000).
57 Yamaguchi M, Watanabe M and Hirai T, ‘Electrical actuation of poly(vinyl
chloride) gel’, Polym. Preprints, Jpn., 48, 2124 (1999).
58 Hirai T, Zheng J, Watanabe M and Shirai H, ‘Electro-active non-ionic gel and its
application’, Proceedings of SPIE, 3987, 281 (2000).
59 Hirai T, Zheng J, Watanabe M, Shirai H and Yamaguchi M, ‘Electroactive
nonionic polymer gel swift bending and crawling motion’, Materials Research
Society Symposium Proceedings, 600, 267—272 (2000).
60 Hirai T, Sadatoh H, Ueda T, Kasazaki T, Kurita Y, Hirai M and Hayashi S,
‘Polyurethane elastomer actuator’, Angew. Makromol. Chem., 240, 221 (1996).
61 Watanabe M, Yokoyama M, Ueda T, Kasazaki T, Hirai M and Hirai T, ‘Bending
deformation of monolayer polyurethane ﬁlm induced by an electric ﬁeld’, Chem.
Lett., 773 (1997).
62 Watanabe M, Suzuki M, Amaike Y and Hirai T, ‘Electric conduction in bending
electrostriction of polyurethanes’, Appl. Phys. Lett., 74, 2717 (1999).
63 Watanabe M, Kato T, Suzuki M, Amaike Y and Hirai T, ‘Bending electrostriction
in polyurethanes containing ions as contaminants or additives’, Jpn. J. Appl. Phys.,
38, Part 2, No. 8A, L872 (1999).
Heat-storage and thermo-regulated
textiles and clothing
3.1 Development introduction
The human body is itself is an automatic thermo-regulated organism. The
body constantly generates heat, CO and H O by the metabolism of food and
muscle activity. The human body controls the release speed of heat by blood
vessel dilatation or constriction, muscle and sweat gland activity, etc., and then
regulates the body temperature.
It has been shown that the most comfortable skin temperature is 33.4 °C.
When the temperature of any part of the skin diﬀers by within 1.5—3.0 °C of this
ideal temperature, the human body is unaware of the warmth or coolness. If
the diﬀerence is more than 4.5 °C, the human body feels discomfort. In
addition, a core body temperature of 36.5 °C is required, and a rise or fall of
1.5 °C can be fatal. A balance between the rates of heat loss and heat generated
must be maintained. When the thermal resistance of their clothing is
insuﬃcient, and a person stays in a relatively low temperature condition for a
long time, the body temperature drops. The human body must produce more
heat by eating more food or increasing exercise. Also, the body will adjust to
the heat loss by constricting the blood capillaries within the skin. Hypothermia
may result, if the core temperature is lower than 35 °C. Conversely, in a hot
environment, the body must cool itself. The body generates heat and the heat
absorbed by the skin from the environment must be dissipated. Under these
conditions the body will dilate the blood capillaries, which enables the
evaporation of water diﬀused from the body interior to increase, thereby
increasing the cooling eﬀect. This action is known as insensible perspiration. If
the environment temperature increases further, the body will activate sweat
glands and evaporate liquid water for increased cooling, known as sensible
perspiration. In some special environments, due to the high temperature or
high thermal resistance of the clothing, hyperthermia can result if the body
fails to dissipate suﬃcient heat.
Heat-storage and thermo-regulated textiles and clothing 35
The traditional heat insulation materials, for example, fabrics such as
cotton, hemp, silk, wool and polyester, polyamide and polyacrylic ﬁbre, etc.
provide a degree of resistance to body heat loss, which is determined by the
number of air pockets present in the fabric. The solar ray selective absorbing
textile that has been manufactured since the late 1980s can absorb the near
infra-red ray in the sun rays, and convert it to heat, thus enhancing the inner
temperature of the clothing. The far infra-red textile that has been produced
since the late 1980s can absorb the body’s irradiated far infra-red ray and turn
it to heat, enhancing thermal resistance. The ultra-violet absorbing and
cool-feeling fabric that has been industrialized since the beginning of the 1990s
can absorb the ultra-violet and reﬂect the near infra-red rays from the sun,
lowering the inner temperature of the clothing. All of these new functional
textiles are one-way thermo-regulated heat insulating materials.
To keep the skin temperature within the 30.4 to 36.4 °C interval, we must put
on or take oﬀ our clothing according to the external temperature. If clothing
could automatically change its thermal resistance according to the temperature,
it could control the speed of heat release, and then regulate the inner
temperature. We would not need to put it on or take it oﬀ very often, and the
proper inner temperature would not only increase body comfort, but also
3.1.2 Development history
The heat-storage and thermo-regulated textiles and clothing are newer
concepts: they are two-way thermo-regulated new products, and have been
studied for more than 30 years. The development history of heat-storage and
thermo- regulated textiles and clothing is outlined in Table 3.1.
Scientists have increasingly been studying the manufacture process and
properties of heat-storage and thermo-regulated textiles and clothing for
several decades. There will be more reports about basic, dynamic thermal
resistance and its applications in the near future.
3.2 Basics of heat-storage materials
There are three types of heat storage: sensible, latent and chemical reaction
heat storage. Latent heat storage is the most important way of storing heat,
and is also called ‘phase change heat storage’. Latent heat-storage materials
have been widely used for about 40 years.
The US National Aeronautics and Space Administration (NASA) accelerated
the application research of latent heat-storage materials for the space
laboratory in the 1960s. They were used to improve the protection of
instruments and astronauts against extreme ﬂuctuations in temperature in